- Nano Express
- Open Access
Effects of CsSnxPb1−xI3 Quantum Dots as Interfacial Layer on Photovoltaic Performance of Carbon-Based Perovskite Solar Cells
Nanoscale Research Letters volume 16, Article number: 74 (2021)
In this work, inorganic tin-doped perovskite quantum dots (PQDs) are incorporated into carbon-based perovskite solar cells (PSCs) to improve their photovoltaic performance. On the one hand, by controlling the content of Sn2+ doping, the energy level of the tin-doped PQDs can be adjusted, to realize optimized band alignment and enhanced separation of photogenerated electron–hole pairs. On the other hand, the incorporation of tin-doped PQDs provided with a relatively high acceptor concentration due to the self-p-type doping effect is able to reduce the width of the depletion region near the back surface of the perovskite, thereby enhancing the hole extraction. Particularly, after the addition of CsSn0.2Pb0.8I3 quantum dots (QDs), improvement of the power conversion efficiency (PCE) from 12.80 to 14.22% can be obtained, in comparison with the pristine device. Moreover, the experimental results are analyzed through the simulation of the one-dimensional perovskite/tin-doped PQDs heterojunction.
In past few years, perovskite materials have been widely applied in solar cells due to their excellent electrical and optical properties, such as suitable bandgap width, large light absorption coefficient and good defect tolerance [1,2,3,4,5,6]. Interface engineering, as a strategy to modify the interface characteristics of thin film devices, has become one of the approaches to improve the performance of perovskite solar cells (PSCs) [7, 8]. Recently, lead-based halide perovskite quantum dots (PQDs) in the form of APbX3 (A = CH3NH3+ (MA+), Cs+; X = Cl−, Br−, I−) are often used as interfacial layers or additives for optimized band alignment thanks to their adjustable band structures [9,10,11,12,13,14,15]. The combination of perovskite absorbers and PQDs is regarded as an effective method for enhanced charge extraction and improved PSC properties.
It is worth noting that most of the relevant researches are based on PSCs with hole-transporting layers (HTLs). In recent years, carbon-based HTL-free PSCs with simple preparation processes and low costs have been given much attention [16,17,18]. Similarly, PQDs can also be used in this PSC structure. However, some other requirements besides band alignment should be taken into consideration. First, the lattice structures of lead-based PQDs are not very stable due to Pb2+ with a large ionic radius reducing the tolerance factor. Therefore, lead-reduced PQDs are promising candidates. Second, because of the lack of HTLs, the hole transport performance is bound to be weakened. Consequently, the added PQDs are required to supply extra free holes, so that photogenerated holes can be smoothly transferred from the perovskite layer to the carbon electrode.
The ion exchange method using metal cations with smaller ionic radii (such as Cu2+, Zn2+, Sn2+, Cd2+) to partially replace Pb2+ has been proven to improve the lattice stability of PQDs [19,20,21]. Among these metal cations, Sn2+ is easily to oxidize to Sn4+, which can introduce self-p-type doping effects to enhance hole transfer [22,23,24]. Particularly, Liu et al. synthesized CsSn0.6Pb0.4I3 quantum dots (QDs) featuring a hole mobility of 40.12 cm2 V−1 s−1 and good stability in the ambient air . Xu and co-workers incorporated CsSnBr3−xIx QDs between the CsPbBr3 perovskite and the carbon electrode to promote charge extraction . Very recently, Duan et al. found that MAPbI3/CsSnI3 heterojunction as the light-harvester in the carbon-based HTL-free PSC could facilitate the hole transfer . Inspired by these above, we propose that tin-doped PQDs with appropriate energy levels and self-p-type doping effects are able to function like HTLs to modify the injection and transport characteristics of holes.
In this work, tin-doped PQDs in the form of CsSnxPb1−xI3 were incorporated between the MAPbI3 perovskite and the carbon electrode to achieve optimized band alignment and improved hole transfer. An increment in power conversion efficiency (PCE) of 11.09%, from 12.80 to 14.22%, could be obtained after the addition of CsSn0.2Pb0.8I3 QDs.
Tin iodide (SnI2; 99.99%) was bought from Youxuan Technology (China). Cesium carbonate (Cs2CO3; 99%), 1-octadecene (ODE; > 90%), oleic acid (OA; 99%), oleylamine (OAM; 80–90%), methyl acetate (MeOAc; 98%) and trioctylphosphine (TOP; 90%) were purchased from Macklin (China). Lead iodide (PbI2; 99.99%) and methylammonium iodide (MAI; 99.5%) were obtained from Xi’an p-OLED (China). Titanium diisopropoxide bis (acetylacetonate; 75%), dimethylsulfoxide (DMSO; 99.9%) and N,N-dimethylformamide (DMF; 99.8%) were purchased from Sigma-Aldrich (US). The TiO2 paste (30NR-D) and the low-temperature carbon electrode paste were obtained from Shanghai MaterWin New Materials (China).
Synthesis and Purification of Tin-Doped PQDs
We adopted a simple mixed-heating procedure to synthesize tin-doped PQDs. Briefly, Cs2CO3, SnI2 and PbI2 with a specific molar ratio (CsSn0.1Pb0.9I3 QDs: 0.037 mmol Cs2CO3, 0.2 mmol PbI2, 0.15 mmol SnI2; CsSn0.2Pb0.8I3 QDs: 0.037 mmol Cs2CO3, 0.2 mmol PbI2, 0.2 mmol SnI2; CsSn0.3Pb0.7I3 QDs: 0.037 mmol Cs2CO3, 0.2 mmol PbI2, 0.25 mmol SnI2) were mixed with 10 mL of ODE, 0.5 mL of OA, 0.5 mL of OAM and 0.5 mL of TOP in a 50-mL three-neck flask. OA, OAM and TOP were utilized to limit the particle size and to passivate the surface defects of tin-doped PQDs. Then, the mixture was stirred and heated at 100 °C for 30 min under nitrogen atmosphere to obtain a red solution, including nano-sized and micron-sized tin-doped perovskites. To extract and purify tin-doped PQDs, 10 mL of MeOAc was added into the red solution, followed by centrifuging at 7000 rpm for 5 min. The supernatant was discarded, and the brown black precipitate was dispersed in 5 mL of hexane. Finally, the brown black solution was centrifuged at 3000 rpm for 5 min, and the red supernatant contained only the tin-doped PQDs.
Fluorine-doped SnO2 (FTO) glasses were washed with water, acetone, isopropanol and ethanol in sequence for 30 min each in an ultrasonic cleaner. After that, the FTO glasses were treated by ultraviolet (UV) for 20 min to remove residual organic solvents. The compact TiO2 (c-TiO2) layer was fabricated on the FTO layer by spin-coating a solution of acetylacetonate (0.1 mL) diluted in ethanol (1.9 mL) with the speed of 4000 rpm for 30 s. Then, the glasses were annealed at 150 °C for 5 min and at 500 °C for 30 min. Subsequently, the mesoporous TiO2 (m-TiO2) layer was obtained by spin-coating a solution of TiO2 paste diluted in ethanol onto the c-TiO2 layer at 3500 rpm for 20 s and annealed at 500 °C for 30 min. The annealing process at 500 °C is to obtain TiO2 layers with improved electron transport performance. Next, to prepare the MAPbI3 precursor solution, PbI2 (0.5 mmol) and MAI (0.5 mmol) were mixed with DMF (300 mg) and DMSO (39 mg). Afterward, the MAPbI3 layer was fabricated by spin-coating the MAPbI3 precursor solution (35 μL) onto the m-TiO2 layer, with the speed of 1000 rpm for 10 s and 4000 rpm for 20 s, followed by heating at 100 °C for 10 min. After that, tin-doped PQDs dispersed in toluene (10 mg mL−1) were spin-coated onto the perovskite layer at 4000 rpm for 30 s and annealed at 90 °C for 5 min to remove the residual toluene. Finally, the carbon electrode paste was screen-printed on the device and annealed at 100 °C for 10 min.
Transmission electron microscope (TEM) images, selected-area electron diffraction (SAED) views and energy-dispersive X-ray spectroscopy (EDS) analyses of tin-doped PQDs were obtained by a field emission high-resolution transmission electron microscope (JEM-2100F, JEOL, Japan) at an accelerating voltage of 200 kV. The valence band (VB) edges of different materials were acquired from an X-ray photoelectron spectrometer (ESCALAB 250Xi, Thermo Fisher Scientific, USA). Absorption and steady-state photoluminescence (PL) characteristics were collected via an UV–visible spectrophotometer (UV-3600, Shimadzu, Japan) and a fluorescence spectrometer (RF-6000, Shimadzu, Japan), respectively. The cross-sectional image of the PSC and the surface morphologies of perovskite films were obtained by a scanning electron microscope (Zeiss Ultra Plus, Zeiss, Germany). Curves of photocurrent density versus on voltage (J–V) were measured by a sourcemeter (2400, Keithley, USA) with a sunlight simulator (Oriel Sol3A, Newport, US), under AM 1.5G simulated illumination (100 mW cm−2). Monochromatic incident photon-to-electron conversion efficiency (IPCE) spectra and electrochemical impedance spectroscopies (EIS) were obtained from an electrochemical workstation (Zahner, Kronach, Germany). Finally, X-ray diffraction (XRD) patterns of perovskite films and PQDs were acquired from an X-ray diffractometer (Empyrean, PANalytical, Netherlands).
Results and Discussion
Three kinds of tin-doped PQDs were studied in this work, including CsSn0.1Pb0.9I3 QDs, CsSn0.2Pb0.8I3 QDs and CsSn0.3Pb0.7I3 QDs. The actual atomic ratios of Sn/(Sn + Pb) in these PQDs were estimated to be 13.03%, 22.12% and 32.57%, respectively (shown in Additional file 1: Fig. S1 and Tables S1–S3). As shown in Fig. 1, blue-shifts of the steady-state PL peak (673 nm, 669 nm and 656 nm in turn) and the edge of Tauc plot (1.79 eV, 1.80 eV and 1.81 eV in turn) were observed with the increase of Sn doping. For many bulk perovskite materials in the form of ABX3 (A = Cs, MA, FA; B = SnxPb1−x; X = Cl, Br, I), the bandgap often exhibits a downward trend with the increase of the x value. That is because the bandgap is determined by the electronegativity of the B-site atom (Pb2+: χ = 1.6; Sn2+: χ = 1.7). However, when it comes to nanocrystals with quantum confinement, the impact of unit cell volume on bandgap matters more. The perovskite bandgap is known to increase with the decrease of the unit cell volume . Therefore, more Sn2+ substitution would further intensify the lattice contraction, which led to the augment of bandgap width, consistent with the reported research . Meanwhile, the larger electronegativity of Sn atom might be the reason why the bandgap did not increase significantly.
The TEM images of these tin-doped PQDs are exhibited in Fig. 2a–c. These tin-doped PQDs were all square, consistent with the theoretical lattice structure of cubic phase. Besides, the average size of each of these three PQDs was about 15 nm, and there was no significant difference. That was because the size was mainly determined by the reaction temperature, which was kept at 100 °C for all the PQDs. Besides, SAED measurements are shown in Fig. 2d–f. By comparing the interplanar spacing values of different diffraction rings with corresponding standard values (CsPbI3 in cubic phase, ICSD, 181288), some crystal planes including (100), (110), (200) and (220) could be identified, which also indicated that these tin-doped PQDs were mostly composed of cubic nanocrystals (NCs) . Moreover, enlarged TEM images shown in Fig. 2g–i are utilized to probe the crystal plane characteristics. The interplanar distances of (200) plane of these tin-doped PQDs were determined to be 0.308 nm, 0.303 nm and 0.296 nm, in turn, which demonstrated that increasing substitution of Pb2+ by Sn2+ led to the lattice shrinkage, in accordance with their optical characteristics mentioned above.
To further study the lattice structures of these tin-doped PQDs, we performed normalized XRD measurements, shown in Fig. 3. According to the standard XRD data of CsPbI3 in orthorhombic and cubic forms [20, 29], the diffraction peaks associated with orthorhombic and cubic phases were marked with “*” and “#,” respectively. As the amount of Sn doping in PQDs increased, the diffraction angle of the peak corresponding to (200) plane slightly increased, implying that the interplanar distance of (200) plane was reduced, in line with the analysis above. Meanwhile, the intensity of the diffraction peak representing orthorhombic phase showed an increasing trend, which indicated that the phase transition process in the PQDs increased. This might be because the increase in the amount of Sn doping would intensify the oxidation reaction of the PQDs in the air, resulting in more Sn vacancies, which may make Pb refill these vacancies to form an unstable perovskite structure.
Optimized band alignment is crucial for enhancing the extraction of photogenerated carriers and suppressing non-radiative recombination [30,31,32,33]. Figure 4 shows the band structures of various materials including FTO, TiO2, MAPbI3, CsSn0.1Pb0.9I3 QDs, CsSn0.2Pb0.8I3 QDs, CsSn0.3Pb0.7I3 QDs and carbon. Corresponding UPS data and Tauc plots are shown in Additional file 1: Fig. S2. It is clear that the valence band (VB) edge of CsSn0.1Pb0.9I3 QDs (− 5.53 eV) or CsSn0.2Pb0.8I3 QDs (− 5.50 eV) was higher than that of MAPbI3 (− 5.54 eV), satisfying the band alignment requirement. It was able to eliminate the large Schottky barrier formed by the MAPbI3/carbon junction, thus enhancing the hole extraction ability (discussed later) . Furthermore, the higher conduction band (CB) edges of these tin-doped PQDs were expected to hinder the flow of electrons from MAPbI3 to the carbon electrode. However, the VB edge of CsSn0.3Pb0.7I3 QDs (− 5.58 eV) was lower than that of MAPbI3, which would block the hole injection, leading to more charge recombination at the interface between MAPbI3 and the PQDs.
Moreover, the VB edge originates from the interactions between Pb (6s) and I (5p) orbitals, which are also determined by the Sn doping amount. On the one hand, the substitution of Pb2+ by Sn2+ will shrink the lattice structure, leading to shorter Pb–I bonds and stronger interactions between Pb and I orbitals, so that the VB tends to shift to a higher energy position . On the other hand, more lattice distortions (transformation from cubic NCs to orthorhombic NCs) will be introduced into the PQDs with excessive Sn2+ substitution, resulting in expanded volume of [PbI6] octahedra and weaker Pb–I interactions, thus moving the VB to a lower energy position . As a result, the VB edge does not vary linearly with the Sn doping of the PQDs. A reasonable Sn doping content is the key to obtaining an appropriate band structure.
Unlike ordinary lead-based PQDs, tin-doped PQDs will partially undergo oxidation in air due to the presence of Sn2+, described by
CsSnxPb1−xI3 can be assumed to be the combination of CsSnI3 and CsPbI3 with a certain molar ratio. Among the compounds, only CsSnI3 participates in the oxidation reaction. Then, this process can be simplified to
In reaction (2), the transformation from CsSnI3 to Cs2SnI6 is regarded as breaking the connections between [SnI6] octahedra. The reason is that CsSnI3 is formed by corner sharing [SnI6] octahedra, while Cs2SnI6 is made up of isolated [SnI6] octahedra . Therefore, these half of Sn atoms do not leave the perovskite lattice. However, the other half of the Sn atoms are oxidized to SnO2, leaving a lot of Sn vacancies in the lattice, which will accept electrons (or supply holes) and act as p-type dopants. It can be described by Eq. (3) as follows:
That is the reason for the self-p-type doping effects of tin-doped PQDs. Accordingly, under the premise that the lattice structure of tin-doped PQDs can be stabilized, the acceptor concentration of the PQDs will increase with the Sn doping amount.
The cross-sectional image of the PSC is shown in Fig. 5a. The widths of FTO layer, m-TiO2 layer and MAPbI3 layer were about 400 nm, 200 nm and 800 nm, respectively. Because of the low concentration of the PQD solution (10 mg mL−1), it was hard to observe a PQD layer that could be distinguished from the underlying MAPbI3 film. To prove the existence of PQDs on MAPbI3, we performed XPS measurement on the film with the structure of FTO/c-TiO2/m-TiO2/MAPbI3/PQDs. The XPS results are shown in Additional file 1: Fig. S3. The elements including Cs, I, Sn and Pb were all detected, demonstrating that there was a PQD layer on the perovskite film. Besides, as shown in Fig. 5b–e, there were many small-sized white PbI2 particles on the original perovskite film, caused by the partial decomposition of the perovskite in the air. After adding tin-doped PQDs, the number of white particles decreased, and the perovskite films exhibited slightly better grain uniformity and compactness than the pristine sample. However, the morphology difference between the various perovskite films was still not obvious. In order to further distinguish their surface characteristics, we performed grazing incidence XRD (GIXRD) patterns of perovskite films with different tin-doped PQDs, exhibited in Fig. 6. The diffraction peak at about 12.7° is associated with PbI2 . After the modification of tin-doped PQDs, the diffraction intensity ratio of PbI2:(110) plane was decreased, suggesting that the decomposition process of the perovskite film was suppressed.
The curves of photocurrent density versus on voltage (J–V) of different PSCs are displayed in Fig. 7a, and photovoltaic parameters including short-circuit current density (Jsc), open-circuit voltage (Voc), fill factor (FF) and PCE are shown in Table 1. The values of Jsc, Voc, FF and PCE of the PSC without modification by tin-doped PQDs were 22.69 mA cm−2, 0.99 V, 56.78% and 12.80%, respectively. For the CsSn0.1Pb0.9I3 QDs-added PSC, various parameters were improved. However, the improvement was not optimal, which might ascribe to the relatively low Sn doping of the PQDs. In contrast, with the incorporation of CsSn0.2Pb0.8I3 QDs, a Jsc of 23.30 mA cm−2, a Voc of 1.05 V, a FF of 57.90% and a PCE of 14.22% could be obtained. The significant increase in each parameter indicated the reduction of non-radiative recombination and the effective extraction of photogenerated holes. Besides, as shown in Additional file 1: Fig. S4, PCE values for 90% of CsSn0.2Pb0.8I3 QDs-added PSCs surpassed 13%, showing good repeatability. For the PSC modified by CsSn0.3Pb0.7I3 QDs, the values of Jsc and FF seriously dropped to 16.82 mA cm−2 and 47.40%, respectively. The lower VB edge of the PQDs would hinder the hole transfer from the MAPbI3 film to the carbon electrode. Furthermore, when the Sn content of PQDs was too high, more Sn vacancies would be introduced, resulting in more phase transformation products with large bandgap widths [29, 35,36,37], thus seriously impeding the transport process of photogenerated carriers.
As described in Fig. 7b, the IPCE spectra in a wavelength range from 350 to 800 nm increased in the order of CsSn0.3Pb0.7I3 QDs-added device < control device < CsSn0.1Pb0.9I3 QDs-added device < CsSn0.2Pb0.8I3 QDs-added device, in agreement with the corresponding trend of Jsc acquired from the J–V curves. It is clear that the difference of these IPCE curves was mainly reflected in the wavelength range from 550 to 800 nm. Tin-doped PQDs added onto the perovskite film would significantly affect the built-in electric field near the back surface of the perovskite (analyzed in detail later). At the same time, the long-wavelength photons were mainly absorbed by the perovskite near the back surface due to their low energy. When these photons were transformed to carriers, their transport properties would be more easily changed by the above-mentioned built-in electric field than those carriers converted from short-wavelength photons.
In addition, EIS measurements, in a frequency range from 4 to 0.2 MHz at a bias of 0.8 V under simulated AM 1.5G radiation, were performed to analyze the charge transport resistance (RCT) and the barrier capacitance (CT) near the carbon electrode, described in Fig. 7c. Corresponding EIS parameters are also shown in Table 1. With the addition of CsSn0.2Pb0.8I3 QDs, the RCT value was reduced, exhibiting promoted hole extraction and decreased energy loss on the back surface of MAPbI3. Furthermore, compared with the pristine and the CsSn0.1Pb0.9I3 QDs-added PSCs, the value of CT increased, so that a shorter depletion width near the back surface of MAPbI3 (WD) could be deduced based on the following formulas, suggesting facilitated hole transfer.
where A is the active area and dQD is the width of the PQD layer. It is worth noting that the contact between MAPbI3 and the PQDs would form a hole depletion region in MAPbI3. Then, the contact between the PQDs and the carbon electrode would generate a Schottky barrier, which led to a hole depletion region in the PQD layer. Both the depletion regions in MAPbI3 and the PQDs contributed to the barrier capacitance value. For the PSC in the presence of CsSn0.3Pb0.7I3 QDs, the lower VB edge of the PQDs allowed more holes to migrate from the PQD layer to the MAPbI3 film. These holes gradually moved away from the MAPbI3/PQDs interface under the isotype heterojunction electric field, thereby increasing the WD. This might be the reason for the low CT value of CsSn0.3Pb0.7I3 QDs-added device.
To get insight on the carrier transfer process, the steady-state PL spectra for the MAPbI3 films with and without tin-doped PQDs were measured. As shown in Fig. 7d, the PL peak intensity at about 775 nm was obviously decreased after the incorporation of CsSn0.1Pb0.9I3 QDs or CsSn0.2Pb0.8I3 QDs. There are two explanations for the weakening of PL intensity: First, the PQDs cause additional non-radiative pathways to capture photogenerated carriers; second, the higher VB edge of PQDs allows more photogenerated holes to migrate to the PQD layer; thus, the number of carriers participating in direct recombination is reduced. However, after adding CsSn0.3Pb0.7I3 QDs with more orthorhombic by-products and lower VB edge, the PL intensity increased, which showed that more carriers were limited in the perovskite film without being trapped by defects. Therefore, the PL quenching of the perovskite film with CsSn0.1Pb0.9I3 QDs or CsSn0.2Pb0.8I3 QDs was caused by the optimized band alignment promoting the hole extraction, instead of interfacial trap-assisted recombination.
In order to further understand the effects of tin-doped PQDs on the hole transport in MAPbI3 films, a one-dimensional MAPbI3/tin-doped PQDs heterojunction model was constructed, shown in Fig. 8a. To simplify the analysis, this structure was regarded as a mutant isotype heterojunction, and MAPbI3 and tin-doped PQDs were determined to be p-type semiconductors. Theoretically, MAPbI3 is a kind of intrinsic semiconductor with low doping concentration. However, in the carbon-based perovskite PSCs with no HTLs, the perovskite layer needs to undergo p-type doping treatment. A small amount of DMSO was added in the precursor of perovskite to form a complex with PbI2, so that there were Pb vacancies in the perovskite, which made the perovskite become a p-type semiconductor. Moreover, Laban and Etgar utilized Mott–Schottky analysis to find that the acceptor concentration of MAPbI3 was 2.14 × 1017 cm−3, belonging to the doping level of p-type materials . The contact of two semiconductors with different Fermi levels would form an electric field from the one with a high Fermi level to the another one with a low Fermi level. Consequently, the p–p isotype heterojunction energy band diagram under the equilibrium condition could be obtained, shown in Fig. 8b. According to the Poisson’s equation, the field continuity condition and the depletion approximation , barrier distributions of the isotype heterojunction were expressed by the following equations:
where q is the elementary charge and εQD and NA_QD are the dielectric coefficient and the acceptor concentration for tin-doped PQDs, respectively. VD_MAPbI3 and VD_QD are the potential difference in MAPbI3 and tin-doped PQDs in turn. EFermi_MAPbI3 and EFermi_QD stand for the Fermi levels of MAPbI3 and tin-doped PQDs, respectively. kB is the Boltzmann constant and T is the room temperature. NC and NV are the effective density of states of electrons in conduction band and the effective density of states of holes in valence band, respectively. Na is the acceptor concentration, ni is the intrinsic carrier concentration and WD is the depletion width in MAPbI3. The simulation results are exhibited in Fig. 8c. As the acceptor concentration of tin-doped PQDs increased, both VD_MAPbI3 and WD showed downward trends, indicating that the hole transfer process in the MAPbI3 film was gradually facilitated. Besides, less electrons would be drifted to the interface between MAPbI3 and the PQD layer to recombine with holes. On the contrary, the direct contact between MAPbI3 and the carbon electrode would generate a large Schottky barrier in MAPbI3, resulting in higher values of VD_MAPbI3 and WD, shown in Fig. 8d. In one word, MAPbI3 films modified by tin-doped PQDs with higher acceptor concentrations would be provided with much enhanced hole transport performance. This simulation result explained why the photovoltaic performance of the CsSn0.2Pb0.8I3 QDs-added PSC was better than the pristine and the CsSn0.1Pb0.9I3 QDs-added devices.
In summary, tin-doped PQDs were added between MAPbI3 and the carbon electrode for enhanced PSC performance, due to their flexible energy levels and self-p-type doping effects. Particularly, with the incorporation of CsSn0.2Pb0.8I3 QDs, the PCE value could be improved from 12.80 to 14.22%, in comparison with the pristine device. It was attributed to the band alignment and the appropriate Sn2+ doping content of the PQDs facilitating the hole extraction. This work is prospected to provide a direction for the interface optimization of carbon-based PSCs based on PQDs.
Availability of data and materials
The datasets used and/or analyzed during the current study are available from the corresponding author on reasonable request.
Perovskite solar cell(s)
Perovskite quantum dot(s)
Power conversion efficiency
- c-TiO2 :
- m-TiO2 :
Transmission electron microscope
Selected area electron diffraction
Energy dispersive X-ray spectroscopy
Incident photon-to-electron conversion
Electrochemical impedance spectroscopy
Rong YG, Hu Y, Mei AY, Tan HR, Saidaminov MI, Seok SI, McGehee MD, Sargent EH, Han HW (2018) Challenges for commercializing perovskite solar cells. Science 361:eaat8235
Liao JF, Wu WQ, Jiang Y, Zhong JX, Wang LZ, Kuang DB (2020) Understanding of carrier dynamics, heterojunction merits and device physics: towards designing efficient carrier transport layer-free perovskite solar cells. Chem Soc Rev 49:354–381
Huang JS, Yuan YB, Shao YC, Yan YF (2017) Understanding the physical properties of hybrid perovskites for photovoltaic applications. Nat Rev Mater 2:17042
Hwang T, Yun AJ, Kim J, Cho D, Kim S, Hong S, Park B (2019) Electronic traps and their correlations to perovskite solar cell performance via compositional and thermal annealing controls. ACS Appl Mater Interfaces 11:6907–6917
Zhou R, Yang Z, Xu JZ, Cao GZ (2018) Synergistic combination of semiconductor quantum dots and organic-inorganic halide perovskites for hybrid solar cells. Coord Chem Rev 374:279–313
Eperon GE, Habisreutinger SN, Leijtens T, Bruijnaers BJ, Van Franeker JJ, DeQuilettes DW, Pathak S, Sutton RJ, Grancini G, Ginger DS, Janssen RAJ, Petrozza A, Snaith HJ (2015) The importance of moisture in hybrid lead halide perovskite thin film fabrication. ACS Nano 9:9380–9393
Meng FN, Liu AM, Gao LG, Cao JM, Yan YL, Wang N, Fan MQ, Wei GY, Ma TL (2019) Current progress in interfacial engineering of carbon-based perovskite solar cells. J Mater Chem A 7:8690–8699
Chen K, Wu P, Yang WQ, Su R, Luo DY, Yang XY, Tu YG, Zhu R, Gong QH (2018) Low-dimensional perovskite interlayer for highly efficient lead-free formamidinium tin iodide perovskite solar cells. Nano Energy 49:411–418
Akin S, Altintas Y, Mutlugun E, Sonmezoglu S (2019) Cesium-lead based inorganic perovskite quantum-dots as interfacial layer for highly stable perovskite solar cells with exceeding 21% efficiency. Nano Energy 60:557–566
Zheng XP, Troughton J, Gasparini N, Lin YB, Wei MY, Hou Y, Liu JK, Song KP, Chen ZL, Yang C, Turedi B, Alsalloum AY, Pan J, Chen J, Zhumekenov AA, Anthopoulos TD, Han Y, Baran D, Mohammed OF, Sargent EH, Bakr OM (2019) Quantum dots supply bulk- and surface-passivation agents for efficient and stable perovskite solar cells. Joule 3:1963–1976
Chen LC, Tien CH, Tseng ZL, Ruan JH (2019) Enhanced efficiency of MAPbI3 perovskite solar cells with FAPbX3 perovskite quantum dots. Nanomaterials 9:121
Gao YB, Wu YJ, Lu HB, Chen C, Liu Y, Bai X, Yang LL, Yu WW, Dai QL, Zhang Y (2019) CsPbBr 3 perovskite nanoparticles as additive for environmentally stable perovskite solar cells with 20.46% efficiency. Nano Energy 59:517–526
Cha MY, Da PM, Wang J, Wang WY, Chen ZH, Xiu FX, Zheng GF, Wang ZS (2016) Enhancing perovskite solar cell performance by interface engineering using CH3NH3PbBr0.9I2.1 quantum dots. J Am Chem Soc 138:8581–8587
Sidhik S, Esparza D, Martínez-Benítez A, Lopez-Luke T, Carriles R, Mora-Sero I, de la Rosa E (2017) Enhanced photovoltaic performance of mesoscopic perovskite solar cells by controlling the interaction between CH3NH3PbI3 films and CsPbX3 perovskite nanoparticles. J Phys Chem C 121:4239–4245
Li B, Zhang YN, Zhang YL, Yin LW (2017) Graded heterojunction engineering for hole-conductor-free perovskite solar cells with high hole extraction efficiency and conductivity. Adv Mater 29:1701221
Chan CY, Wang YY, Wu GW, Diau EWG (2016) Solvent-extraction crystal growth for highly efficient carbon-based mesoscopic perovskite solar cells free of hole conductors. J Mater Chem A 4:3872–3878
Sheng YS, Mei AY, Liu SA, Duan M, Jiang P, Tian CB, Xiong YL, Rong YG, Han HW, Hu Y (2018) Mixed (5-AVA)xMA1−xPbI3−y(BF4)y perovskites enhance the photovoltaic performance of hole- conductor-free printable mesoscopic solar cells. J Mater Chem A 6:2360–2364
Xiong YL, Liu Y, Lan K, Mei AY, Sheng YS, Zhao DY, Han HW (2018) Fully printable hole-conductor-free mesoscopic perovskite solar cells based on mesoporous anatase single crystals. New J Chem 42:2669–2674
Van der Stam W, Geuchies JJ, Altantzis T, Van den Bos KHW, Meeldijk JD, Van Aert S, Bals S, Vanmaekelbergh D, De Mello DC (2017) Highly emissive divalent-ion-doped colloidal CsPb1−xMxBr3 perovskite nanocrystals through cation exchange. J Am Chem Soc 139:4087–4097
Zhang JB, Zhang LW, Cai P, Xue XG, Wang MK, Zhang J, Tu GL (2019) Enhancing stability of red perovskite nanocrystals through copper substitution for efficient light-emitting diodes. Nano Energy 62:434–441
Vitoreti ABF, Agouram S, de la Fuente MS, Muñoz-Sanjose V, Schiavon MA, Mora-Sero I (2018) Study of the partial substitution of Pb by Sn in Cs–Pb–Sn–Br nanocrystals owing to obtaining stable nanoparticles with excellent optical properties. J Phys Chem C 122:14222–14231
Gupta S, Cahen D, Hodes G (2018) How SnF2 impacts the material properties of lead-free tin perovskites. J Phys Chem C 122:13926–13936
Mosconi E, Umari P, De Angelis F (2015) Electronic and optical properties of mixed Sn–Pb organohalide perovskites: a first principles investigation. J Mater Chem A 3:9208–9215
Chung I, Song JH, Im J, Androulakis J, Malliakas CD, Li H, Freeman AJ, Kenney JT, Kanatzidis MG (2012) CsSnI3: semiconductor or metal? High electrical conductivity and strong near-infrared photoluminescence from a single material. High hole mobility and phase-transitions. J Am Chem Soc 134:8579–8587
Liu F, Ding C, Zhang YH, Ripolles TS, Kamisaka T, Toyoda T, Hayase S, Minemoto T, Yoshino K, Dai SY, Yanagida M, Noguchi H, Shen Q (2017) Colloidal synthesis of air-stable alloyed CsSn1−xPbxI3 perovskite nanocrystals for use in solar cells. J Am Chem Soc 139:16708–16719
Xu HZ, Duan JL, Zhao YY, Jiao ZB, He BL, Tang QW (2018) 9.13%-efficiency and stable inorganic CsPbBr3 solar cells. Lead-free CsSnBr3−xIx quantum dots promote charge extraction. J Power Sources 399:76–82
Duan QQ, Ji JY, Hong X, Fu YC, Wang CY, Zhou K, Liu XQ, Yang H, Wang ZY (2020) Design of hole-transport-material free CH3NH3PbI3/CsSnI3 all-perovskite heterojunction efficient solar cells by device simulation. Sol Energy 201:555–560
Zhang XL, Cao WY, Wang WG, Xu B, Liu S, Dai HT, Chen SM, Wang K, Sun XW (2016) Efficient light-emitting diodes based on green perovskite nanocrystals with mixed-metal cations. Nano Energy 30:511–516
Swarnkar A, Marshall AR, Sanehira EM, Chernomordik BD, Moore DT, Christians JA, Chakrabarti T, Luther JM (2016) Quantum dot-induced phase stabilization of a-CsPbI3 perovskite for high-efficiency photovoltaics. Science 354:92–95
Minemoto T, Murata M (2014) Impact of work function of back contact of perovskite solar cells without hole transport material analyzed by device simulation. Curr Appl Phys 14:1428–1433
Tian CB, Mei AY, Zhang SJ, Tian HR, Liu S, Qin F, Xiong YL, Rong YG, Hu Y, Zhou YH, Xie SY, Han HW (2018) Oxygen management in carbon electrode for high-performance printable perovskite solar cells. Nano Energy 53:160–167
Jeon NJ, Na H, Jung EH, Yang TL, Lee YG, Kim G, Shin HW, Seok SI, Lee J, Seo J (2018) A fluorene-terminated hole-transporting material for highly efficient and stable perovskite solar cells. Nat Energy 3:682–689
Li C, Wang FZ, Xu J, Yao JX, Zhang B, Zhang CF, Xiao M, Dai SY, Li YF, Tan ZA (2015) Efficient perovskite/fullerene planar heterojunction solar cells with enhanced charge extraction and suppressed charge recombination. Nanoscale 7:9771–9778
Song JX, Bian J, Zheng EQ, Wang XF, Tian WJ, Miyasaka T (2015) Efficient and environmentally stable perovskite solar cells based on ZnO electron collection layer. Chem Lett 44:610–612
Sanehira EM, Marshall AR, Christians JA, Harvey SP, Ciesielski PN, Wheeler LM, Schulz P, Lin LY, Beard MC, Luther JM (2017) Enhanced mobility CsPbI3 quantum dot arrays for record-efficiency, high-voltage photovoltaic cells. Sci Adv 3:eaao4204
Akkerman QA, Park S, Radicchi E, Nunzi F, Mosconi E, De Angelis F, Brescia R, Rastogi P, Prato M, Manna L (2017) Nearly monodisperse insulator Cs4PbX6 (X = Cl, Br, I) nanocrystals, their mixed halide compositions, and their transformation into CsPbX3 nanocrystals. Nano Lett 17:1924–1930
De Weerd C, Lin JH, Gomez L, Fujiwara Y, Suenaga K, Gregorkiewicz T (2017) Hybridization of single nanocrystals of Cs4PbBr6 and CsPbBr3. J Phys Chem C 121:19490–19496
Laban WA, Etgar L (2013) Depleted hole conductor-free lead halide iodide heterojunction solar cells. Energy Environ Sci 6:3249–3253
Kumar RC (1968) On the solution of Poisson equation for an isotype heterojunction under zero-current condition. Solid State Electron 11:543–551
This work was supported by the National Natural Science Foundation of China (NSFC) (11704293, 11974266) and the Fundamental Research Funds for the Central Universities under Grant WUT (2020IB022).
The authors declare that they have no competing interests.
Springer Nature remains neutral with regard to jurisdictional claims in published maps and institutional affiliations.
. EDS mappings of different tin-doped PQDs under HAADF STEM patterns. a CsSn0.1Pb0.9I3 QDs, b CsSn0.2Pb0.8I3 QDs, c CsSn0.3Pb0.7I3 QDs. Fig. S2. UPS data and Tauc plots for a CsSn0.1Pb0.9I3 QDs, b CsSn0.2Pb0.8I3 QDs, c CsSn0.3Pb0.7I3 QDs and d MAPbI3. The valence band (VB) edges were calculated by EVB = − (21.21 eV − ECut-off + ELow-binding). Then, the conduction band (CB) edges were calculated by ECB = EVB + Eg. Fig. S3. XPS measurement on the film with the structure of FTO/c-TiO2/m-TiO2/MAPbI3/PQDs. Fig. S4. Bar charts indicating photovoltaic parameters of ten CsSn0.2Pb0.8I3 QDs-added devices at the PQD concentration of 10 mg mL−1. Fig. S5. Error bars of photovoltaic parameters for different PSCs. Fig. S6. Normalized PCE values for CsSn0.2Pb0.8I3 QDs-added and the pristine devices at 60% humidity in room temperature. Table S1. EDS chemical composition analysis for CsSn0.1Pb0.9I3 QDs. Table S2. EDS chemical composition analysis for CsSn0.2Pb0.8I3 QDs. Table S3. EDS chemical composition analysis for CsSn0.3Pb0.7I3 QDs. Table S4. Photovoltaic parameters of different PSCs. Table S5. Photovoltaic parameters of CsSn0.2Pb0.8I3 QDs-added PSCs under different concentrations of the PQD solution.
About this article
Cite this article
Zhang, C., He, Z., Luo, X. et al. Effects of CsSnxPb1−xI3 Quantum Dots as Interfacial Layer on Photovoltaic Performance of Carbon-Based Perovskite Solar Cells. Nanoscale Res Lett 16, 74 (2021). https://doi.org/10.1186/s11671-021-03533-y
- Tin-doped perovskite quantum dots
- Photovoltaic performance
- Carbon-based perovskite solar cells